Resistance spot welding typically employs electrical power in the form of direct current, alternating current, medium frequency half-wave direct current, or high-frequency half wave direct current. If excessive heat is applied or applied too quickly, or if the force between the base materials is too low, or the coating is too thick or too conductive, then the molten area may extend to the exterior of the work pieces, escaping the containment force of the electrodes (often up to 30,000 psi). This burst of molten metal is called expulsion, and when this occurs the metal will be thinner and have less strength than a weld with no expulsion. The common method of checking a weld's quality is a peel test. An alternative test is the restrained tensile test, which is much more difficult to perform, and requires calibrated equipment. Because both tests are destructive in nature (resulting in the loss of salable material), non-destructive methods such as ultrasound evaluation are in various states of early adoption by many OEMs. The advantages of the method include efficient energy use, limited workpiece deformation, high production rates, easy automation, and no required filler materials. When high strength in shear is needed, spot welding is used in preference to more costly mechanical fastening, such as riveting. While the shear strength of each weld is high, the fact that the weld spots do not form a continuous seam means that the overall strength is often significantly lower than with other welding methods, limiting the usefulness of the process. It is used extensively in the automotive industry— cars can have several thousand spot welds. A specialized process, called shot welding, can be used to spot weld stainless steel. There are three basic types of resistance welding bonds: solid state, fusion, and reflow braze. In a "solid state bond", also called a thermo-compression bond, dissimilar materials with dissimilar grain structure, e.g. molybdenum to tungsten, are joined using a very short heating time, high weld energy, and high force. There is little melting and minimum grain growth, but a definite bond and grain interface. Thus the materials actually bond while still in the solid state. The bonded materials typically exhibit excellent shear and tensile strength, but poor peel strength. In a "fusion bond", either similar or dissimilar materials with similar grain structures are heated to the melting point (liquid state) of both. The subsequent cooling and combination of the materials forms a “nugget” alloy of the two materials with larger grain growth.